Materials Science Medicine
Chemistry,1970-2014-Chemistry-2013.jsonl.gz.gz
Chemistry
841a1b77dd70ab00d2f9cd58e7f0ba634e4aa9df
An assessment of zinc oxide nanosheets as a selective adsorbent for cadmium

Zinc oxide nanosheet is assessed as a selective adsorbent for the detection and adsorption of cadmium using simple eco-friendly extraction method. Pure zinc oxide nanosheet powders were characterized using field emission scanning electron microscopy, energy dispersive spectroscopy, X-ray diffraction, X-ray photoelectron spectroscopy, and Fourier transform infrared spectroscopy. The zinc oxide nanosheets were applied to different metal ions, including Cd(II), Cu(II), Hg(II), La(III), Mn(II), Pb(II), Pd(II), and Y(III). Zinc oxide nanosheets were found to be selective for cadmium among these metal ions when determined by inductively coupled plasma-optical emission spectrometry. Moreover, adsorption isotherm data provided that the adsorption process was mainly monolayer on zinc oxide nanosheets.


Background
With the development of industry and economy, environmental problem becomes more and more serious day by day [1][2][3]. Due to certain man-made activities, numerous hazardous compounds and heavy metals are introduced into the environment which is a concerning matter for monitoring agencies and regulation authorities [4][5][6]. Among these pollutants, toxic metals are the most sever pollutants and main environmental threat which instigate too many serious public health and cost-cutting problems [7,8]. Cadmium is known to be as highly toxic as probably carcinogenic for humans and is listed as the sixth most poisonous substance jeopardizing human health. Cadmium is introduced into water bodies from different sources, for example, smelting, metal plating, cadmiumnickel batteries, phosphate fertilizers, mining, pigments, stabilizers, alloy industries, and sewage sludge. The harmful effects of Cd(II) involve a number of acute and chronic disorders such as gastrointestinal irritation, vomiting, abdominal pain, diarrhea, renal damage, emphysema, hypertension, and testicular atrophy [9,10]. Therefore, separation and determination of Cd(III) in different matrices have continued to be of import.
In addition, the development of simple, rapid, and efficient methods has become of interest for monitoring metal ions in the environment. Several analytical methods have been applied to analyze metal ions in aqueous solutions [7,8]. However, analytical methods cannot directly measure metal ions, in particular at ultra-trace concentration, in aqueous systems due to the lack of sensitivity and selectivity of these methods. Therefore, an efficient separation procedure is usually required prior to the determination of noble metals for sensitive, accurate, and interference-free determination of noble metals.
Several analytical methods have been utilized for separation of analyte of interest, including liquid/liquid extraction, ion exchange, coprecipitation, cloud-point extraction, and solid-phase extraction (SPE) [11,12]. SPE is considered to be one of the most powerful techniques because it minimizes solvent usage and exposure, disposal costs, and extraction time for sample preparation. Several adsorbents have appeared because of the popularity of SPE for selective extraction of analytes such polymers, silica, carbon nanotube, etc. [7,8].
Nanoscience and technology have attracted significant attention due to its potential application in various fields and especially in metal ion adsorption [13,14]. ZnO, a versatile material, emerges as a challenging prospect in the field of nanotechnology. Nanosized ZnO has been widely used as a catalyst [14], gas sensor [15,16], active filler for rubber and plastic, ultraviolet (UV) absorber in cosmetics, and antivirus agent in coating [17,18] and has more potential application in building functional electronic devices with special architecture and distinctive optoelectronic properties.
In this investigation, we synthesized ZnO nanosheets by stirring method and characterized by X-ray diffraction patterns (XRD), field emission scanning electron microscopy (FESEM), Fourier transform infrared spectroscopy (FT-IR), X-ray photoelectron spectroscopy (XPS), and energy dispersive spectroscopy (EDS). ZnO nanosheets were applied to investigate their utility and the analytical efficiency as adsorbent on the selectivity and adsorption capacity of Cd(II). The selectivity of ZnO nanosheets toward eight metal ions, including Cd(II), Cu(II), Hg(II), La(III), Mn(II), Pb(II), Pd(II), and Y(III), was investigated in order to study the effectiveness of ZnO nanosheets on the adsorption of selected metal ions. Based on the selectivity study, the ZnO nanosheets attained the highest selectivity toward Cd(II). Static uptake capacity of ZnO nanosheets for Cd(II) was found to be 97.36 mg g −1 . Adsorption isotherm data of Cd(II) with ZnO nanosheets were well fit with the Langmuir adsorption isotherm, strongly confirming that the adsorption process was mainly monolayer on homogeneous adsorbent surfaces.

Chemicals and reagents
Zinc nitrate, sodium hydroxide, mercuric nitrate, lanthanum nitrate, palladium nitrate, and yttrium nitrate were purchased from Sigma-Aldrich (Milwaukee, WI, USA). Stock standard solutions of 1,000 mgL −1 Cd(II), Cu(II), Mn(II), and Pb(II) were also obtained from Sigma-Aldrich. All reagents used were of high purity and of spectral purity grade, and doubly distilled deionized water was used throughout.

Preparation of ZnO nanosheets
ZnO nanosheets were synthesized by thermal stirring method in which 0.1 M of zinc nitrate aqueous solution was titrated with 0.1 M solution of NaOH till pH reached above 10 and stirred at 70°C for overnight. White product was washed and dried. The dried product was calcined at 450°C for 4 h.

Characterization
The morphology of the synthesized product was studied at 15 kV using a JEOL Scanning Electron Microscope (JSM-7600 F, Akishima-shi, Japan). XRD was taken with a computer-controlled RINT 2000, Rigaku diffractometer (Shibuya-ku, Japan) using the Ni-filtered Cu-Kα radiation (λ = 0.15405 nm). FT-IR spectrum was recorded in the range of 400 to 4,000 cm −1 on PerkinElmer (spectrum 100, Waltham, MA, USA) FT-IR spectrometer. XPS spectrum was recorded in the range of 0 to 1,350 eV by using Thermo Scientific K-Alpha KA1066 spectrometer (Schwerte, Germany).
Samples preparation and procedure for metal uptake study

Results and discussion
Structural characterization FESEM was used for the general structural characterization of the calcined products and demonstrated in Figure 2. It is clear from the images that the synthesized product is grown in high density. The calcined product possess sheet like structure and average thickness of the grown nanosheets is approximately 10 nm.
The chemical composition of the synthesized nanosheets was studied by energy dispersive spectroscopy (EDS), and the results were depicted in Figure 3. The EDS did not show any element except zinc and oxygen which suggest that the synthesized nanosheets are pure ZnO.
To check the crystallinity of the synthesized ZnO nanosheets, X-ray diffraction technique was used, and results are shown in Figure 4a. A series of characteristic peaks were obtained which are responsible for wurtzite hexagonal ZnO. X-ray diffraction confirms that the obtained nanomaterial is pure ZnO with wurtzite hexagonal phase [19]. Figure 4b shows the typical FT-IR spectra of the ZnO nanomaterial measured in the range of 420 to 4,000 cm −1 . The appearance of a sharp band at 495.18 cm −1 in the FT-IR spectrum is indication of ZnO nanosheets which is due to Zn-O stretching vibration [19]. The absorption peaks at 3,477 and 1,612 cm −1 are caused by the O-H stretching of the absorbed water molecules from the environment [20].
XPS was analyzed for synthesized nanosheets and described in Figure 5. XPS peaks for calcined nanosheets observed at 531.1 for O 1 s, 1,022.0 eV for Zn 2p 3/2 , and 1,045.0 eV for Zn 2p 1/2 which are comparable to the literature values [21] which suggest pure ZnO nanosheets.

Metal uptake Selectivity study of ZnO nanosheets
Selectivity of the newly synthesized ZnO nanosheets toward different metal ions was investigated based on the basis of calculated distribution coefficient of ZnO nanosheets. The distribution coefficient (K d ) can be obtained from the following equation [22]: where C o and C e refer to the initial and final concentrations before and after filtration with ZnO nanosheets, respectively, V is the volume (mL), and m is the weight

Static adsorption capacity
For determination of the static uptake capacity of Cd(II) on ZnO nanosheet adsorbent, 25 mL Cd(II) sample solutions with different concentrations (0 to 150 mg L −1 ) were adjusted to pH 5.0 and individually mixed with 25 mg ZnO nanosheets ( Figure 6). These mixtures were mechanically shaken for 1 h at room temperature. Static adsorption capacity was obtained using Equation 2 as follows: where q e represents the adsorbed metal ion by the adsorbent (mg g −1 ), C o and C e are the initial and equilibrium concentrations of metal ion in solution (mg L −1 ),  respectively, V is the volume (L), and m is the weight of adsorbent (g). Figure 7a displays the metal uptake capacity of ZnO nanosheets for Cd(II) obtained from the experiment of adsorption isotherm. Adsorption capacity of ZnO nanosheets for Cd(II) was determined to be 97.36 mg g −1 . Reported adsorption capacity in this study was found to be comparable with those previously reported for Cd(II) (4.92 [23], 9.39 [24], 84.30 [25], 57.90 [26], 95.20 [27], 123.65 mg g −1 [28]) in other studies. In comparison with the adsorption capacity of ZnO nanosheets toward Cd(II), uptake capacities of other nanostructures for Cd (II) were also previously reported. For example, the adsorption capacity of Cd(II) on MnO 2 functionalized multi-walled carbon nanotubes was determined to be 41.60 mg g −1 by Luo et al. [29]. In addition, adsorption capacities of nano B 2 O 3 /TiO 2 composite material and nanocrystallite hydroxyapatite for Cd(II) were previously evaluated and reported to be 49.00 [30] and 142.86 mg g −1 [31]. As discussed above, the adsorption capacity of nanostructures for Cd(II) may vary. However, ZnO nanosheets possess the most important property in its high efficiency and selectivity for Cd(II). Thus, the high selectivity of ZnO nanosheets enables the method for accurate and precise determination of Cd(II) in complex matrices.

Adsorption isotherm models
Experimental equilibrium adsorption data were analyzed using different models in order to develop an equation that accurately represents the results. Langmuir equation is based on an assumption of a monolayer adsorption onto a completely homogeneous surface with a finite number of identical sites and a negligible interaction between the adsorbed molecules. The Langmuir adsorption isotherm model is governed by the following relation [7]: where C e corresponds to the equilibrium concentrations of Cd(II) ion in solution (mg mL −1 ) and q e is the adsorbed metal ion by the adsorbate (mg g −1 ). The symbols Q o and b refer to Langmuir constants related to adsorption capacity (mg g −1 ) and energy of adsorption (L mg −1 ), respectively. These constants can be determined from a  linear plot of C e /q e against C e with a slope and intercept equal to 1/Q o and 1/Q o b, respectively. Moreover, the essential characteristics of Langmuir adsorption isotherm can be represented in terms of a dimensionless constant separation factor or equilibrium parameter, R L , which is defined as R L = 1/(1 + bC o ), where b is the Langmuir constant (indicates the nature of adsorption and the shape of the isotherm); C o the initial concentration of the analyte. The R L value indicates the type of the isotherm, and R L values between 0 and 1 represent a favorable adsorption [8].
The experimental isotherm data were best fit with the Langmuir equation (Figure 7b) based on the least square fit, confirming the validity of Langmuir adsorption isotherm model for the adsorption process. Consequently, adsorption isotherm data suggested that the adsorption process was mainly monolayer on a homogeneous adsorbent surface. Langmuir constants Q o and b are found to be 99.60 mg g −1 and 0.28 L mg −1 , respectively. The correlation coefficient obtained from the Langmuir model is found to be R 2 = 0.989 for adsorption of Cd(II) on ZnO nanosheets. Moreover, the Cd(II) adsorption capacity (99.60 mg g −1 ) calculated from Langmuir equation was consistent with that (97.36 mg g −1 ) of the experimental isotherm study. The R L value of Cd(II) adsorption on the ZnO nanosheets is 0.03, supporting a highly favorable adsorption process based on the Langmuir classical adsorption isotherm model.

Conclusions
ZnO nanosheets were synthesized by low-temperature eco-friendly method and evaluated their efficiency for selective adsorption and determination of Cd(II) in aqueous solution. Reasonable static adsorption capacities of 97.36 mg g −1 for ZnO nanosheet adsorbent were achieved for Cd(II) in aqueous solution. Adsorption isotherm data of Cd(II) were well fit with the Langmuir classical adsorption isotherm model. Thus, the method may play an important role for using it as an effective approach for a selective adsorption and determination of Cd(II) in complex matrices for a range of several applications.